#------------------------------------------------------------------------------
#$Date: 2016-03-26 22:39:59 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180514 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/83/7218382.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7218382
loop_
_publ_author_name
'Pan, ShiLie'
'Wang, Zheng'
'Jing, Qun'
'Zhang, Min'
'Dong, Xiaoyu'
'Yang, Zhihua'
_publ_section_title
;
 Cs4Mg3CaF12: Structural Transition Derived from the Partial Substitution
 of Mg2+ with Ca2+
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C4RA07819E
_journal_year                    2014
_chemical_formula_sum            'Ca Cs4 F12 Mg3'
_chemical_formula_weight         872.65
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   6.2196(9)
_cell_length_b                   6.2196(9)
_cell_length_c                   29.812(9)
_cell_measurement_reflns_used    1531
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.54
_cell_measurement_theta_min      3.84
_cell_volume                     998.7(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0183
_diffrn_reflns_av_sigmaI/netI    0.0112
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       37
_diffrn_reflns_limit_l_min       -38
_diffrn_reflns_number            2049
_diffrn_reflns_theta_full        27.56
_diffrn_reflns_theta_max         27.56
_diffrn_reflns_theta_min         3.84
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    11.512
_exptl_absorpt_correction_T_max  0.746
_exptl_absorpt_correction_T_min  0.645
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   face-indexed
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.353
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1152
_exptl_crystal_size_max          0.145
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.097
_refine_diff_density_max         0.546
_refine_diff_density_min         -0.576
_refine_diff_density_rms         0.093
_refine_ls_extinction_coef       0.00103(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.202
_refine_ls_matrix_type           full
_refine_ls_number_parameters     27
_refine_ls_number_reflns         329
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.202
_refine_ls_R_factor_all          0.0123
_refine_ls_R_factor_gt           0.0110
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0087P)²+3.0175P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0247
_refine_ls_wR_factor_ref         0.0256
_reflns_number_gt                313
_reflns_number_total             329
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4ra07819e2.cif
_cod_data_source_block           3333
_cod_original_sg_symbol_H-M      R-3m
_cod_database_code               7218382
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'-x, -x+y, -z'
'x-y, -y, -z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+1/3'
'-x+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, -y+1/3, -z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+2/3'
'-x+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, -y+2/3, -z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'x, x-y, z'
'-x+y, y, z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cs1 Cs 0.0000 0.0000 0.131513(10) 0.01625(11) Uani 1 6 d S
Cs2 Cs 0.6667 0.3333 0.050278(10) 0.01415(11) Uani 1 6 d S
Mg1 Mg 0.3333 0.6667 0.1667 0.0110(5) Uani 1 12 d S
Mg2 Mg 0.3333 0.6667 0.07507(5) 0.0102(3) Uani 1 6 d S
Ca1 Ca 0.0000 0.0000 0.0000 0.0114(3) Uani 1 12 d S
F1 F 0.17524(15) 0.3505(3) 0.04161(5) 0.0173(4) Uani 1 2 d S
F2 F 0.0570(3) 0.52851(15) 0.12313(5) 0.0149(4) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
F2 Cs1 F2 119.371(8) 2 .
F2 Cs1 F2 119.371(8) 2 3
F2 Cs1 F2 119.371(8) . 3
F2 Cs1 F2 165.49(6) 2 2_665
F2 Cs1 F2 48.55(6) . 2_665
F2 Cs1 F2 71.02(6) 3 2_665
F2 Cs1 F2 48.55(6) 2 3_455
F2 Cs1 F2 71.02(6) . 3_455
F2 Cs1 F2 165.49(6) 3 3_455
F2 Cs1 F2 119.371(8) 2_665 3_455
F2 Cs1 F2 71.02(6) 2 1_545
F2 Cs1 F2 165.49(6) . 1_545
F2 Cs1 F2 48.55(6) 3 1_545
F2 Cs1 F2 119.371(8) 2_665 1_545
F2 Cs1 F2 119.371(8) 3_455 1_545
F2 Cs1 F2 97.17(3) 2 26_445
F2 Cs1 F2 126.873(15) . 26_445
F2 Cs1 F2 56.86(5) 3 26_445
F2 Cs1 F2 97.17(3) 2_665 26_445
F2 Cs1 F2 126.873(15) 3_455 26_445
F2 Cs1 F2 56.86(5) 1_545 26_445
F2 Cs1 F2 126.873(15) 2 27
F2 Cs1 F2 56.86(5) . 27
F2 Cs1 F2 97.17(3) 3 27
F2 Cs1 F2 56.86(5) 2_665 27
F2 Cs1 F2 97.17(3) 3_455 27
F2 Cs1 F2 126.873(15) 1_545 27
F2 Cs1 F2 70.62(5) 26_445 27
F2 Cs1 F2 56.86(5) 2 25_455
F2 Cs1 F2 97.17(3) . 25_455
F2 Cs1 F2 126.873(15) 3 25_455
F2 Cs1 F2 126.873(15) 2_665 25_455
F2 Cs1 F2 56.86(5) 3_455 25_455
F2 Cs1 F2 97.17(3) 1_545 25_455
F2 Cs1 F2 70.62(5) 26_445 25_455
F2 Cs1 F2 70.62(5) 27 25_455
F2 Cs1 F1 53.98(4) 2 2
F2 Cs1 F1 89.50(3) . 2
F2 Cs1 F1 113.66(4) 3 2
F2 Cs1 F1 113.66(4) 2_665 2
F2 Cs1 F1 53.98(4) 3_455 2
F2 Cs1 F1 89.50(3) 1_545 2
F2 Cs1 F1 143.224(19) 26_445 2
F2 Cs1 F1 143.223(19) 27 2
F2 Cs1 F1 102.97(4) 25_455 2
F2 Cs1 F1 89.50(3) 2 3
F2 Cs1 F1 113.66(4) . 3
F2 Cs1 F1 53.98(4) 3 3
F2 Cs1 F1 89.50(3) 2_665 3
F2 Cs1 F1 113.66(4) 3_455 3
F2 Cs1 F1 53.98(4) 1_545 3
F2 Cs1 F1 102.97(4) 26_445 3
F2 Cs1 F1 143.224(19) 27 3
F2 Cs1 F1 143.224(19) 25_455 3
F1 Cs1 F1 59.83(5) 2 3
F2 Cs1 F1 113.66(4) 2 .
F2 Cs1 F1 53.98(4) . .
F2 Cs1 F1 89.50(3) 3 .
F2 Cs1 F1 53.98(4) 2_665 .
F2 Cs1 F1 89.50(3) 3_455 .
F2 Cs1 F1 113.66(4) 1_545 .
F2 Cs1 F1 143.224(19) 26_445 .
F2 Cs1 F1 102.97(4) 27 .
F2 Cs1 F1 143.223(19) 25_455 .
F1 Cs1 F1 59.83(5) 2 .
F1 Cs1 F1 59.83(5) 3 .
F2 Cs2 F2 74.08(5) 1_655 3
F2 Cs2 F2 74.08(5) 1_655 2_665
F2 Cs2 F2 74.08(5) 3 2_665
F2 Cs2 F1 94.59(3) 1_655 2_655
F2 Cs2 F1 56.57(4) 3 2_655
F2 Cs2 F1 130.48(4) 2_665 2_655
F2 Cs2 F1 56.57(4) 1_655 1_655
F2 Cs2 F1 94.59(3) 3 1_655
F2 Cs2 F1 130.48(4) 2_665 1_655
F1 Cs2 F1 63.16(6) 2_655 1_655
F2 Cs2 F1 130.48(4) 1_655 3
F2 Cs2 F1 56.57(4) 3 3
F2 Cs2 F1 94.59(3) 2_665 3
F1 Cs2 F1 56.38(6) 2_655 3
F1 Cs2 F1 119.322(8) 1_655 3
F2 Cs2 F1 56.57(4) 1_655 3_665
F2 Cs2 F1 130.48(4) 3 3_665
F2 Cs2 F1 94.59(3) 2_665 3_665
F1 Cs2 F1 119.322(8) 2_655 3_665
F1 Cs2 F1 56.38(6) 1_655 3_665
F1 Cs2 F1 169.91(6) 3 3_665
F2 Cs2 F1 130.48(4) 1_655 .
F2 Cs2 F1 94.59(3) 3 .
F2 Cs2 F1 56.57(4) 2_665 .
F1 Cs2 F1 119.322(8) 2_655 .
F1 Cs2 F1 169.91(6) 1_655 .
F1 Cs2 F1 63.16(6) 3 .
F1 Cs2 F1 119.322(8) 3_665 .
F2 Cs2 F1 94.59(3) 1_655 2_665
F2 Cs2 F1 130.48(4) 3 2_665
F2 Cs2 F1 56.57(4) 2_665 2_665
F1 Cs2 F1 169.91(6) 2_655 2_665
F1 Cs2 F1 119.322(8) 1_655 2_665
F1 Cs2 F1 119.322(8) 3 2_665
F1 Cs2 F1 63.16(6) 3_665 2_665
F1 Cs2 F1 56.38(6) . 2_665
F2 Cs2 F1 115.25(4) 1_655 21_655
F2 Cs2 F1 115.25(4) 3 21_655
F2 Cs2 F1 167.80(4) 2_665 21_655
F1 Cs2 F1 58.81(5) 2_655 21_655
F1 Cs2 F1 58.81(5) 1_655 21_655
F1 Cs2 F1 85.07(3) 3 21_655
F1 Cs2 F1 85.07(3) 3_665 21_655
F1 Cs2 F1 113.14(2) . 21_655
F1 Cs2 F1 113.14(2) 2_665 21_655
F2 Cs2 F1 167.80(4) 1_655 20
F2 Cs2 F1 115.25(4) 3 20
F2 Cs2 F1 115.25(4) 2_665 20
F1 Cs2 F1 85.07(3) 2_655 20
F1 Cs2 F1 113.14(2) 1_655 20
F1 Cs2 F1 58.81(5) 3 20
F1 Cs2 F1 113.14(2) 3_665 20
F1 Cs2 F1 58.81(5) . 20
F1 Cs2 F1 85.07(3) 2_665 20
F1 Cs2 F1 54.42(5) 21_655 20
F2 Cs2 F1 115.25(4) 1_655 19_665
F2 Cs2 F1 167.80(4) 3 19_665
F2 Cs2 F1 115.25(4) 2_665 19_665
F1 Cs2 F1 113.14(2) 2_655 19_665
F1 Cs2 F1 85.07(3) 1_655 19_665
F1 Cs2 F1 113.14(2) 3 19_665
F1 Cs2 F1 58.81(5) 3_665 19_665
F1 Cs2 F1 85.07(3) . 19_665
F1 Cs2 F1 58.81(5) 2_665 19_665
F1 Cs2 F1 54.42(5) 21_655 19_665
F1 Cs2 F1 54.42(5) 20 19_665
F2 Mg1 F2 81.49(7) . 3_565
F2 Mg1 F2 81.49(7) . 2_665
F2 Mg1 F2 81.49(7) 3_565 2_665
F2 Mg1 F2 180.0 . 25_565
F2 Mg1 F2 98.51(7) 3_565 25_565
F2 Mg1 F2 98.51(7) 2_665 25_565
F2 Mg1 F2 98.51(7) . 27
F2 Mg1 F2 179.998(1) 3_565 27
F2 Mg1 F2 98.51(7) 2_665 27
F2 Mg1 F2 81.49(7) 25_565 27
F2 Mg1 F2 98.51(7) . 26_455
F2 Mg1 F2 98.51(7) 3_565 26_455
F2 Mg1 F2 180.0 2_665 26_455
F2 Mg1 F2 81.49(7) 25_565 26_455
F2 Mg1 F2 81.49(7) 27 26_455
F1 Mg2 F1 96.71(8) 3_565 .
F1 Mg2 F1 96.71(8) 3_565 2_665
F1 Mg2 F1 96.71(8) . 2_665
F1 Mg2 F2 92.28(5) 3_565 3_565
F1 Mg2 F2 166.45(10) . 3_565
F1 Mg2 F2 92.28(5) 2_665 3_565
F1 Mg2 F2 92.28(5) 3_565 .
F1 Mg2 F2 92.28(5) . .
F1 Mg2 F2 166.45(10) 2_665 .
F2 Mg2 F2 77.20(8) 3_565 .
F1 Mg2 F2 166.45(10) 3_565 2_665
F1 Mg2 F2 92.28(5) . 2_665
F1 Mg2 F2 92.28(5) 2_665 2_665
F2 Mg2 F2 77.20(8) 3_565 2_665
F2 Mg2 F2 77.20(8) . 2_665
F1 Ca1 F1 180.00(7) 19 .
F1 Ca1 F1 92.73(6) 19 21
F1 Ca1 F1 87.27(6) . 21
F1 Ca1 F1 87.27(6) 19 3
F1 Ca1 F1 92.73(6) . 3
F1 Ca1 F1 180.00(7) 21 3
F1 Ca1 F1 92.73(6) 19 20
F1 Ca1 F1 87.27(6) . 20
F1 Ca1 F1 92.73(6) 21 20
F1 Ca1 F1 87.27(6) 3 20
F1 Ca1 F1 87.27(6) 19 2
F1 Ca1 F1 92.73(6) . 2
F1 Ca1 F1 87.27(6) 21 2
F1 Ca1 F1 92.73(6) 3 2
F1 Ca1 F1 180.00(8) 20 2
Mg2 F1 Ca1 177.05(10) . .
Mg2 F1 Cs2 89.07(3) . 1_455
Ca1 F1 Cs2 91.19(3) . 1_455
Mg2 F1 Cs2 89.07(3) . .
Ca1 F1 Cs2 91.19(3) . .
Cs2 F1 Cs2 169.91(6) 1_455 .
Mg2 F1 Cs2 88.49(7) . 19_665
Ca1 F1 Cs2 88.56(5) . 19_665
Cs2 F1 Cs2 94.93(3) 1_455 19_665
Cs2 F1 Cs2 94.93(3) . 19_665
Mg2 F1 Cs1 94.80(7) . .
Ca1 F1 Cs1 88.15(5) . .
Cs2 F1 Cs1 85.14(3) 1_455 .
Cs2 F1 Cs1 85.14(3) . .
Cs2 F1 Cs1 176.71(6) 19_665 .
Mg1 F2 Mg2 85.00(7) . .
Mg1 F2 Cs2 175.16(8) . 1_455
Mg2 F2 Cs2 90.16(6) . 1_455
Mg1 F2 Cs1 91.23(3) . .
Mg2 F2 Cs1 97.23(3) . .
Cs2 F2 Cs1 89.38(3) 1_455 .
Mg1 F2 Cs1 91.23(3) . 1_565
Mg2 F2 Cs1 97.23(3) . 1_565
Cs2 F2 Cs1 89.38(3) 1_455 1_565
Cs1 F2 Cs1 165.49(6) . 1_565
Mg1 F2 Cs1 90.78(6) . 25_455
Mg2 F2 Cs1 175.78(8) . 25_455
Cs2 F2 Cs1 94.06(5) 1_455 25_455
Cs1 F2 Cs1 82.83(3) . 25_455
Cs1 F2 Cs1 82.83(3) 1_565 25_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cs1 F2 3.1349(5) 2
Cs1 F2 3.1349(5) .
Cs1 F2 3.1349(5) 3
Cs1 F2 3.1349(5) 2_665
Cs1 F2 3.1349(5) 3_455
Cs1 F2 3.1349(5) 1_545
Cs1 F2 3.1503(17) 26_445
Cs1 F2 3.1503(17) 27
Cs1 F2 3.1503(17) 25_455
Cs1 F1 3.2783(18) 2
Cs1 F1 3.2783(18) 3
Cs1 F1 3.2783(18) .
Cs2 F2 3.0229(16) 1_655
Cs2 F2 3.0229(16) 3
Cs2 F2 3.0229(16) 2_665
Cs2 F1 3.1219(5) 2_655
Cs2 F1 3.1219(5) 1_655
Cs2 F1 3.1219(5) 3
Cs2 F1 3.1219(5) 3_665
Cs2 F1 3.1219(5) .
Cs2 F1 3.1219(5) 2_665
Cs2 F1 3.2256(18) 21_655
Cs2 F1 3.2256(18) 20
Cs2 F1 3.2256(18) 19_665
Mg1 F2 1.9747(16) .
Mg1 F2 1.9747(16) 3_565
Mg1 F2 1.9747(16) 2_665
Mg1 F2 1.9747(16) 25_565
Mg1 F2 1.9747(16) 27
Mg1 F2 1.9748(16) 26_455
Mg2 F1 1.9737(18) 3_565
Mg2 F1 1.9737(18) .
Mg2 F1 1.9737(18) 2_665
Mg2 F2 2.066(2) 3_565
Mg2 F2 2.066(2) .
Mg2 F2 2.066(2) 2_665
Ca1 F1 2.2589(16) 19
Ca1 F1 2.2589(16) .
Ca1 F1 2.2589(16) 21
Ca1 F1 2.2589(16) 3
Ca1 F1 2.2589(16) 20
Ca1 F1 2.2589(16) 2
F1 Cs2 3.1219(5) 1_455
F1 Cs2 3.2256(18) 19_665
F2 Cs2 3.0229(16) 1_455
F2 Cs1 3.1349(5) 1_565
F2 Cs1 3.1503(17) 25_455
